Dielectric phase transition of an A<sub>2</sub>BX<sub>4</sub>-type perovskite with a pentahedral to octahedral transformation.
Chai, Siqian; Xiong, Jianbo; Zheng, Yongshen; Shi, Rongchao; Xu, Jialiang; Dalton transactions (Cambridge, England : 2003) 49 (2020) 2218–2224; doi:10.1039/c9dt04270a

data_7703294
_publ_section_title
;
 Dielectric phase transition of an A<sub>2</sub>BX<sub>4</sub>-type
 perovskite with a pentahedral to octahedral transformation.
;
_journal_issue                   7
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              2218
_journal_page_last               2224
_journal_paper_doi               10.1039/c9dt04270a
_journal_volume                  49
_journal_year                    2020
_chemical_formula_sum            'C10 H24 Br4 N2 Pb'
_chemical_formula_weight         699.14
_space_group_crystal_system      orthorhombic
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2020-01-10 deposited with the CCDC.	2020-01-15 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.15(5)
_cell_length_b                   24.90(7)
_cell_length_c                   6.200(10)
_cell_measurement_reflns_used    5221
_cell_measurement_temperature    210(2)
_cell_measurement_theta_max      53.12
_cell_measurement_theta_min      6.30
_cell_volume                     1876(10)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2014/4 (Sheldrick, 2014)'
_diffrn_ambient_temperature      210(2)
_diffrn_measured_fraction_theta_full 0.973
_diffrn_measured_fraction_theta_max 0.973
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           GaK\a
_diffrn_radiation_wavelength     1.34139
_diffrn_reflns_av_unetI/netI     0.0634
_diffrn_reflns_Laue_measured_fraction_full 0.973
_diffrn_reflns_Laue_measured_fraction_max 0.973
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       28
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            1531
_diffrn_reflns_point_group_measured_fraction_full 0.973
_diffrn_reflns_point_group_measured_fraction_max 0.973
_diffrn_reflns_theta_full        51.237
_diffrn_reflns_theta_max         51.237
_diffrn_reflns_theta_min         3.088
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    18.290
_exptl_absorpt_correction_T_max  0.7519
_exptl_absorpt_correction_T_min  0.3137
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.476
_exptl_crystal_description       plate
_exptl_crystal_F_000             1280
_exptl_crystal_size_max          0.210
_exptl_crystal_size_mid          0.180
_exptl_crystal_size_min          0.150
_refine_diff_density_max         5.263
_refine_diff_density_min         -3.561
_refine_diff_density_rms         0.491
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.071
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     137
_refine_ls_number_reflns         1531
_refine_ls_number_restraints     288
_refine_ls_restrained_S_all      0.977
_refine_ls_R_factor_all          0.1512
_refine_ls_R_factor_gt           0.1272
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1080P)^2^+298.2738P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.3062
_refine_ls_wR_factor_ref         0.3235
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1187
_reflns_number_total             1531
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c9dt04270a2.cif
_cod_data_source_block           platon_tw
_cod_depositor_comments
'Adding full bibliography for 7703293--7703296.cif.'
_cod_original_cell_volume        1875(9)
_cod_database_code               7703294
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_min   0.114
_shelx_estimated_absorpt_t_max   0.170
_shelx_res_checksum              97142